VOLUME 78, NUMBER 21

PHYSICAL REVIEW LETTERS

26 MAY 1997

Stabilization of Ternary Compounds via Ordered Arrays of Defect Pairs S. B. Zhang, Su-Huai Wei, and Alex Zunger National Renewable Energy Laboratory, Golden, Colorado 80401 (Received 17 January 1997) 2 First-principles calculations show that the defect pair s2VCu 1 In1 Cu d in CuInSe2 has an unusually low formation energy, due both to the relative ease of forming Cu vacancies sVCu d and to the attractive 2 21 and InCu . The defect pair is predicted to be electrically inactive. This explains interactions between VCu the surprising electrical tolerance of CuInSe2 to its huge s,1%d concentration of native defects. An attractive interaction among the defect pairs is further predicted to lead to a crystallographic ordering of the pairs, explaining the observed, but hitherto surprising, structures CuIn5Se8, CuIn3Se5, Cu2In4Se7, etc. [S0031-9007(97)03239-0]

PACS numbers: 61.72.Bb, 61.72.Ji, 71.20.Nr

The field of condensed matter physics of perfect crystalline lattices owes its relevance to experiment to the fact that the formation of native defects usually costs significant energy. Thus, perfect crystalline lattices should exist, at least in principle. One may, however, contemplate the possibility of the spontaneous formation of defect complexes in crystalline lattices. If DHf sa, qd is the formation energy of a point defect of type a (vacancy, antisite, interstitial, . . . ) in charge state q, then, even if DHf sa, qd . 0 for a single defect, it is possible that the formation energy of a pair, a complex, or an array of interacting defects, DHf sa 1 bd fDHf sad 1 DHf sbdg 1 dHint 1 dHord ,

(1)

could be very small, or even negative. This could happen if the (positive) formation energy of two isolated defects fDHf sad 1 DHf sbdg is small, but the attractive interaction energy dHint between the components of a defect pair, and/or the pair-pair ordering energy dHord are strongly stabilizing. First-principles calculations have shown, however, that the lowest formation energy of a 21 single, interacting defect pair—fGa22 As 1 AsGa g in GaAs 22 21 [1,2], and fVZn 1 Zni g in ZnSe [3]—is still as high as 2–3 eV. Thus defect pairs are unlikely to form spontaneously in ordinary binary semiconductors. We have identified a semiconductor system—the ternary chalcopyrites of the AI BIII X2VI type [4] (e.g., CuInSe2), where the formation of ordered arrays [5] of defect pairs can be made exothermic even at low temperatures. Using the local density approximation (LDA), our total energy calculations show the following: (i) The formation of a single noninteracting (neutral) 0 d plus one defect pair made of two Cu vacancies s2VCu 0 In-on-Cu antisite sInCu d costs only 4.26 eV. (ii) The 0 strong interaction dHint 23.45 eV between 2VCu 0 and InCu reduces the formation energy to only 0.81 eV, significantly lower than that for the lowest-energy pairs in GaAs or ZnSe. Furthermore, (iii) repeating periodically 2 21 m units of s2VCu 1 InCu d for every n unit of CuInSe2, 0031-9007y97y78(21)y4059(4)$10.00

nsCuInSe2 d 1 msInd ! Cusn23mdInsn1md Se2n 1 3msCud 1 DHf sn, md ,

(2)

where m 1, 2, 3, . . ., and n 3, 4, 5, . . ., and where (In) and (Cu) denote In and Cu in their respective equilibrium chemical reservoirs, reduces the energy further by dHord , 20.8 eVypair. Thus, the energy DHf sn, md need to form such “defect pair arrays” from CuInSe2 is close to zero and can even be made negative by a proper choice of the reservoir energies. (iv) The charge2 1 In21 compensated defect pair s2VCu Cu d is found to have no electric energy levels in the band gap. Our findings can potentially explain two long-standing puzzles in the chalcopyrite material system [6,7]: First, Cu2 Se 1 In2 Se3 are known [6] to form a series of compounds such as CuIn5Se8, CuIn3Se5, Cu2In4Se7, . . . , with hitherto unexplained Cu:In:Se ratios. We suggest that the extraordinar2 0 1 In21 ily low formation energy of a single pair s2VCu Cu d and the significant pair-pair ordering energy lead to the formation of “ordered defect arrays” [viz., Eq. (2)], such as CuIn5Se8 (n 4, m 1), CuIn3Se5 (n 5, m 1), Cu2In4Se7 (n 7, m 1), etc. Second, while, in ordinary semiconductors, polycrystallinity leads to a high concentration of electrically active defects that have a detrimental effect on the performance of optoelectronic devices, polycrystalline CuInSe2 is as good an electronic material as its single-crystal counterpart [7], even though it has a huge amount of structural defects. We explain 2 and In21 this by the attractive interaction between VCu Cu , leading to an effective electric annihilation of these recombination centers. The formation energy DHf sa, qd of defect a in charge state q depends on the Fermi energy eFa (where a denotes absolute values), as well as on the atomic chemical potentials ma . In CuInSe2, DHf sa, qd Esa, qd 2 EsCuInSe2 d 1 nCu maCu a a 1 nIn mIn 1 nSe mSe 1 qeFa ,

(3)

where Esa, qd is the total energy of a supercell containing a defect of type a and charge q, EsCuInSe2 d is the total © 1997 The American Physical Society

4059

VOLUME 78, NUMBER 21

PHYSICAL REVIEW LETTERS

26 MAY 1997

energy for the same supercell in the absence of the defect, the n’s are the numbers of Cu, In, and Se atoms, and q is the number of electrons, transferred from the defect-free supercell to the reservoirs in forming the defect cell. We will not consider Se-related defects in this study so we take nSe 0. Denoting DEsa, qd Esa, qd 2 EsCuInSe2 d 1 nCu msolid Cu solid 1 nIn mIn 1 qEV ,

(4)

DHf sa, qd DEsa, qd 1 nCu mCu 1 nIn mIn 1 qeF , (5) and where eF eFa 2 EV , mCu maCu 2 msolid Cu , . Here E is defined as E mIn maIn 2 msolid V V In sNd sN21d sNd 1 eVBM , where E0 ; EsCuInSe2 d is E0 2 E1 the ground state total energy of the N-electron neutral sN21d is the total energy of the CuInSe2 with system and E1 a hole in the VBM and an electron in the reservoir with an energy eVBM equal to the valence-band maximum (VBM) eigenvalue. There are some thermodynamic limits to sm, eF d: eF is bound between the VBM and the conduction-band minimum (CBM), and hmCu , mIn j are bound by (i) the values that will cause precipitation of solid elemental Cu, In, and Se, so mCu # 0,

mIn # 0,

mSe # 0 ,

(6)

(ii) by the values that maintain a stable CuInSe2 compound, so mCu 1 mIn 1 2mSe DHf sCuInSe2 d ,

(7)

where DHf sCuInSe2 d 21.97 eV is the calculated formation energy of solid CuInSe2, and (iii) by the values that will cause formation of binaries, so 2mIn 1 3mSe # DHf sIn2 Se3 d , 2mCu 1 mSe # DHf sCu2 Sed ,

(8)

where our calculated DHf stetragonal In2 Se3 d 22.07 eV [8] and DHf sCu2 Sed 20.31 eV, respectively. Figure 1 gives the calculated “stability triangle” in the twodimensional smCu , mIn d plane as defined by Eqs. (6) and (7). The vertices are A (the Cu-rich and In-rich limit), B (the Cu-poor and In-rich limit), and C (the Cu-rich and In-poor limit). Equation (8) defines the regions where In2Se3 and Cu2Se are stable. We calculated DHf sa, qd for a VCu , VIn , InCu , CuIn , and interstitial Cu sCui d using a 32-atom supercell and a uniform jellium background where q fi 0. The total energies are calculated using the LDA as implemented by the general potential linearized augmented plane wave (LAPW) method [9]. We used Ceperley-Alder exchange correlation potential [10] as parametrized by Perdew and Zunger [11]. The core states are treated relativistically, while the valence states are treated nonrelativistically. The LDA error on the band gap is corrected by adding a constant potential to the conduction states so that the band 4060

FIG. 1. The calculated stability triangle of the Cu-In-Se systems [Eqs. (6) and (7)] in the hmCu , mIn j plane. The vertices correspond to (A) Cu-rich, In-rich; (B) Cu-poor, In-rich; and (C) Cu-rich, In-poor, respectively.

gap of CuInSe2 matches the experimental value of 1.04 eV [7]. The atomic positions were fully relaxed for the q 0 charge state, but no further relaxation was attempted for q fi 0. We estimated that the error in our calculated defect formation energies is 60.2 eV per defect. Figure 2 shows the defect formation energy DHf sa, qd for single defects as a function of the electron Fermi energy eF at the chemical potential values A, B, and C denoted in Fig. 1. The solid dots denote points where the slope of DHf sa, qd vs q changes; the corresponding value of eF is the defect transition energy Ea sqyq0 d. Figure 2 shows the following: (i) The formation energies of single neutral defects 0 d in CuInSe2 are extraordinarily low, e.g., DHf sVCu 0 21.2 eV (at B) and DHf sCuIn d 20.3 eV (at C). In

FIG. 2. Formation energies [Eq. (5)] of VCu , InCu , and CuIn as a function of the electron Fermi energy eF at chemical potentials A, B, and C as shown in Fig. 1. Charge state q determines the slope of each line segment. The shaded area highlights negative formation energies.

VOLUME 78, NUMBER 21

PHYSICAL REVIEW LETTERS

particular, the formation energy of the neutral Cu vacancy is significantly lower than the vacancy formation energies for cations in II-VI’s. There are two reasons (“ionic” and “covalent”) for this. First, Cu is monovalent, while cations in II-VI’s are divalent, so the pointion (Madelung) contribution to the removal energy of the cation is larger in II-VI’s. Second, the covalent Cu-Se bond is easier to break than that of Zn-Se because the Cu 4p energy is higher than the Zn 4p energy (thus the Cu-Se bond is less covalent). Furthermore, the formation of sp 3 hybrids costs more energy in CuInSe2. This is so because the high-lying Cu 3d orbital (relative to the Zn 3d orbital) repels the Se 4p orbital to higher energy [12], thus raising the Se 4s ! 4p promotion energy. (ii) Several low-energy point defects of opposite charges exist at the same eF and m. This allows the formation of charge-compensated defect pairs of low energies, listed in Table I. Notable in Table I is the low formation energy 0 0 1 InCu d of 21.74 eV at point B. neutral pair s2VCu The formation energy of the noninteracting defect pairs can be lowered considerably through interaction and ordering: (a) Interaction: The interaction energy dHint between the component of an isolated pair [Eq. (1)] is calculated as the difference DHf sa 1 bd 2 DHf sad 2 DHf sbd (using the 32-atom supercell [13]). Total energy minimization shows that (Table I) dHint is 24 to 21 eV. We have analyzed the physical origins of dHint by breaking it 2 21 1 InCu d, for example, into recognizable terms. For s2VCu we find dHint 23.45 eV with three contributions: (i) the transfer of two electrons from the high-energy donor level to low-energy acceptor level releases ,21.0 eV (see Fig. 2) and produces charged defect components, (ii) a strong electrostatic attraction between the ensuing charged defects releases ,21.5 eV, and (iii) atomic relaxations upon pairing releases 20.9 eV. The equilibrium geometry of the pair is shown in Fig. 3, where two Cu vacancies are fcc nearest neighbors to the InCu antisite. This arrangement maximizes the point-ion interactions. Furthermore, it lowers the strain: The atomic radius of In is about 23% larger than that of Cu, therefore the pairing of InCu with Cu vacancies reduces the strain energy.

26 MAY 1997

(b) Ordering: Defect pairs whose components are charged may order in the lowest electrostatic Madelung energy configuration. Indeed, we found that the directly calculated LAPW ordering energies scale with the Madelung ordering energies of the same charged defect pair arrays. We thus searched for the lowest-energy array made of 2 21 1 InCu d units by considering a large number of s2VCu ordered configurations, using a simple point-ion model. The lowest energy configuration found forms a tetragonal superstructure with lattice vectors along the f110g, f112g, and f112g directions, respectively, resulting in a Cu 2 VCu 2 InCu 2 VCu f110g superlattice (which can also be viewed as f001g stacking of the vacancy planes). The pair-pair ordering energy dHord sn, m 1d (Table I) for the most stable structure was then calculated by subtracting from the LAPW energy of the defect array the en2 ergy of the isolated s2VCu 1 In21 Cu d pair. dHord sn, m 1d depends on n with an average value of 20.8 eV. We can see from Table I that the sum of interaction and ordering energies dHint 1 dHord of Eq. (1) for the de2 fect pair array s2VCu 1 In21 Cu d is about 24.25 eV, which cancels most of the (positive) formation energy of the iso0 0 d 1 DHf sInCu d 4.26 eV lated, neutral pair: 2DHf sVCu at A. Table II shows the formation energies DHf sn, m 2 21 1d for a few ordered arrays of s2VCu 1 InCu d for the chemical potentials A, B, and C, respectively. We see that a spontaneous formation of stable defect arrays is predicted. The arrows in Fig. 1 point to the chemical potential domains where these ordered defect arrays will be thermodynamically stable. The results of Table II and Fig. 1 can be used to understand the peculiar Cu-In-Se structures known [6] to exist. They can be divided into two classes: those that are on the Cu2Se-In2Se3 tie line [i.e., the compound that can be written as sCu2 Sedx sIn2 Se3 d12x with 0 # x # 1] and those that are not. We predict the stability of all observed tieline compounds as resulting from the repetition of m units

TABLE I. The calculated formation energies DHnon DHf sad 1 DHf sbd (in eV) of noninteracting neutral defects, the intrapair interaction energies dHint , and the pair-pair ordering energies dHord sn, m 1d at chemical potentials A, B, and C as shown in Fig. 1. 0 0 0 0 0 2VCu 1 InCu Cu0In 1 2Cu0i VCu 1 Cu0i InCu 1 CuIn

DHnon dHint dHord

4.26sAd 21.74sBd 6.26sCd 23.45 ,20.8

6.07sAd 12.07sBd 4.07sCd 22.61 ···

2.93sAd 2.93sBd 2.93sCd 21.13 ···

4.47sAd 4.47sBd 4.47sCd 23.67 ···

2 FIG. 3. The calculated structural model for the s2VCu 1 In21 Cu d defect pair.

4061

VOLUME 78, NUMBER 21

PHYSICAL REVIEW LETTERS

TABLE II. Calculated formation energies DHf sn, m 1d DHnon smd 1 dHint 1 dHord sn, m 1d [Eq. (2)] (in eV) of the 2 21 ordered arrays of n units of s2VCu 1 InCu d for every m unit of CuInSe2. dHord sn, m 1d are 20.76, 20.78, and 20.79 eV for n 4, 5, and 6, respectively, while dHint and DHnon smd are taken from the first column of Table I. CuIn5Se8 CuIn3Se5 Cu3In7Se12

n

mA

mB

mC

4 5 6

0.05 0.03 0.02

25.95 25.97 25.98

2.05 2.03 2.02

2 of s2VCu 1 In21 Cu d for every n unit of CuInSe2. These are CuIn5Se8 (n 4, m 1), CuIn3Se5 (n 5, m 1), Cu2In4Se7 (n 7, m 1), Cu3In5Se9 (n 9, m 1), and Cu7In19Se32 (n 16, m 3). Electron diffraction data on CuIn3Se5 [14] suggest f001g stacking of the vacancies, in agreement with our calculations. There are three off-the-tie-line compounds that are observed [6] but not accounted for by the above argument: CuIn7Se12, Cu4In9Se16, and Cu3In6Se11. In light of the low formation energy of neutral Cu vacancy (Fig. 2), we can rationalize the stabilities of these three compounds as emerging from the creation of 2, 1, and 1 Cu vacancies per molecule in the (tie-line) compounds Cu3In7Se12 (n 6, m 1), Cu5In9Se16 (n 8, m 1), and Cu4In6Se11 (n 11, m 1), respectively. To understand why CuInSe2 exhibits a surprising electric tolerance to its .1% structural point defects, we calculated the electronic structure of an isolated, interacting 2 1 In21 s2VCu Cu d pair. All the deep defect levels of VCu and InCu (which act as the recombination centers) are removed from the band gap due to pairing. We also find that, when the defect array orders, the (LDA-corrected) band gaps of the “ordered defect compounds” CuIn5Se8, CuIn3Se5, and Cu3In7Se12 are 1.38, 1.29, and 1.23 eV, respectively, all larger than the 1.04 eV band gap of CuInSe2. This explains the surprising electrical tolerance of nonstoichiometric CuInSe2 to its structural defects [7]. In summary, the key factors that stabilize spontaneous defect-pair formation and ordering in CuInSe2 are (i) the ability to form charge-compensating defects solely on the cation sublattices (thus, the need for two heterovalent cations), (ii) the low metal vacancy formation energy

4062

26 MAY 1997

(thus, the need for low-valent cations with possibly active d orbitals), and (iii) the large interdefect electrostatic interactions (thus, the need for partially ionic systems). This work was supported by the U.S. Department of Energy, DOE-EERE under Contract No. DE-AC3683CH10093.

[1] S. B. Zhang and J. E. Northrup, Phys. Rev. Lett. 67, 2339 (1991). [2] G. A. Baraff and M. Schluter, Phys. Rev. B 33, 7346 (1986). [3] D. B. Laks et al., Phys. Rev. B 45, 10 965 (1992); C. Van De Walle (private communication). [4] J. L. Shay and J. H. Wernick, Ternary Chalcopyrite Semiconductors (Pergamon, Oxford, 1975). [5] Composition-preserving antisite pairs are trivial cases, where the formation of an array does not cost any energy, e.g., zinc-blende GaAs can be viewed as a 50%-50% solid made of antisite pairs GaAs 1 AsGa . Here, we will discuss cases other than the antisite pair arrays. [6] P. Villars and L. D. Calvert, Pearson’s Handbook of Crystallographic Data for Intermetallic Phases (ASM International, Materials Park, Ohio, 1991), p. 2884. [7] Copper Indium Diselenide for Photovoltaic Applications, edited by T. J. Coutts, L. L. Kazmerski, and S. Wagner (Elsevier, Amsterdam, 1986). [8] Here, we will not consider hexagonal In2Se3, despite the fact that its calculated energy is about 1.1 eV lower. We expect that decomposition of (tetragonal) CuInSe2 produces initially tetragonal In2Se3 which is inhibited by an activation barrier from transforming into the hexagonal phase. [9] S.-H. Wei and H. Krakauer, Phys. Rev. Lett. 55, 1200 (1985). [10] D. M. Ceperly and B. J. Alder, Phys. Rev. Lett. 45, 566 (1980). [11] J. P. Perdew and A. Zunger, Phys. Rev. B 23, 5048 (1981). [12] S.-H. Wei and A. Zunger, Phys. Rev. B 37, 8958 (1988). [13] We assume that the long-range Coulomb interactions 2 and In21 among charged VCu Cu dominate the cell-cell interaction. Using a dielectric constant of e 16 [7], 2 1 In21 the cell-cell interaction of s2VCu Cu d in the 32-atom supercell is estimated to be less than 60.1 eV. [14] H. Z. Xiao, L.-Chung Yang, and A. Rockett, J. Appl. Phys. 76, 1503 (1994).

PHYSICAL REVIEW LETTERS

26 MAY 1997

Stabilization of Ternary Compounds via Ordered Arrays of Defect Pairs S. B. Zhang, Su-Huai Wei, and Alex Zunger National Renewable Energy Laboratory, Golden, Colorado 80401 (Received 17 January 1997) 2 First-principles calculations show that the defect pair s2VCu 1 In1 Cu d in CuInSe2 has an unusually low formation energy, due both to the relative ease of forming Cu vacancies sVCu d and to the attractive 2 21 and InCu . The defect pair is predicted to be electrically inactive. This explains interactions between VCu the surprising electrical tolerance of CuInSe2 to its huge s,1%d concentration of native defects. An attractive interaction among the defect pairs is further predicted to lead to a crystallographic ordering of the pairs, explaining the observed, but hitherto surprising, structures CuIn5Se8, CuIn3Se5, Cu2In4Se7, etc. [S0031-9007(97)03239-0]

PACS numbers: 61.72.Bb, 61.72.Ji, 71.20.Nr

The field of condensed matter physics of perfect crystalline lattices owes its relevance to experiment to the fact that the formation of native defects usually costs significant energy. Thus, perfect crystalline lattices should exist, at least in principle. One may, however, contemplate the possibility of the spontaneous formation of defect complexes in crystalline lattices. If DHf sa, qd is the formation energy of a point defect of type a (vacancy, antisite, interstitial, . . . ) in charge state q, then, even if DHf sa, qd . 0 for a single defect, it is possible that the formation energy of a pair, a complex, or an array of interacting defects, DHf sa 1 bd fDHf sad 1 DHf sbdg 1 dHint 1 dHord ,

(1)

could be very small, or even negative. This could happen if the (positive) formation energy of two isolated defects fDHf sad 1 DHf sbdg is small, but the attractive interaction energy dHint between the components of a defect pair, and/or the pair-pair ordering energy dHord are strongly stabilizing. First-principles calculations have shown, however, that the lowest formation energy of a 21 single, interacting defect pair—fGa22 As 1 AsGa g in GaAs 22 21 [1,2], and fVZn 1 Zni g in ZnSe [3]—is still as high as 2–3 eV. Thus defect pairs are unlikely to form spontaneously in ordinary binary semiconductors. We have identified a semiconductor system—the ternary chalcopyrites of the AI BIII X2VI type [4] (e.g., CuInSe2), where the formation of ordered arrays [5] of defect pairs can be made exothermic even at low temperatures. Using the local density approximation (LDA), our total energy calculations show the following: (i) The formation of a single noninteracting (neutral) 0 d plus one defect pair made of two Cu vacancies s2VCu 0 In-on-Cu antisite sInCu d costs only 4.26 eV. (ii) The 0 strong interaction dHint 23.45 eV between 2VCu 0 and InCu reduces the formation energy to only 0.81 eV, significantly lower than that for the lowest-energy pairs in GaAs or ZnSe. Furthermore, (iii) repeating periodically 2 21 m units of s2VCu 1 InCu d for every n unit of CuInSe2, 0031-9007y97y78(21)y4059(4)$10.00

nsCuInSe2 d 1 msInd ! Cusn23mdInsn1md Se2n 1 3msCud 1 DHf sn, md ,

(2)

where m 1, 2, 3, . . ., and n 3, 4, 5, . . ., and where (In) and (Cu) denote In and Cu in their respective equilibrium chemical reservoirs, reduces the energy further by dHord , 20.8 eVypair. Thus, the energy DHf sn, md need to form such “defect pair arrays” from CuInSe2 is close to zero and can even be made negative by a proper choice of the reservoir energies. (iv) The charge2 1 In21 compensated defect pair s2VCu Cu d is found to have no electric energy levels in the band gap. Our findings can potentially explain two long-standing puzzles in the chalcopyrite material system [6,7]: First, Cu2 Se 1 In2 Se3 are known [6] to form a series of compounds such as CuIn5Se8, CuIn3Se5, Cu2In4Se7, . . . , with hitherto unexplained Cu:In:Se ratios. We suggest that the extraordinar2 0 1 In21 ily low formation energy of a single pair s2VCu Cu d and the significant pair-pair ordering energy lead to the formation of “ordered defect arrays” [viz., Eq. (2)], such as CuIn5Se8 (n 4, m 1), CuIn3Se5 (n 5, m 1), Cu2In4Se7 (n 7, m 1), etc. Second, while, in ordinary semiconductors, polycrystallinity leads to a high concentration of electrically active defects that have a detrimental effect on the performance of optoelectronic devices, polycrystalline CuInSe2 is as good an electronic material as its single-crystal counterpart [7], even though it has a huge amount of structural defects. We explain 2 and In21 this by the attractive interaction between VCu Cu , leading to an effective electric annihilation of these recombination centers. The formation energy DHf sa, qd of defect a in charge state q depends on the Fermi energy eFa (where a denotes absolute values), as well as on the atomic chemical potentials ma . In CuInSe2, DHf sa, qd Esa, qd 2 EsCuInSe2 d 1 nCu maCu a a 1 nIn mIn 1 nSe mSe 1 qeFa ,

(3)

where Esa, qd is the total energy of a supercell containing a defect of type a and charge q, EsCuInSe2 d is the total © 1997 The American Physical Society

4059

VOLUME 78, NUMBER 21

PHYSICAL REVIEW LETTERS

26 MAY 1997

energy for the same supercell in the absence of the defect, the n’s are the numbers of Cu, In, and Se atoms, and q is the number of electrons, transferred from the defect-free supercell to the reservoirs in forming the defect cell. We will not consider Se-related defects in this study so we take nSe 0. Denoting DEsa, qd Esa, qd 2 EsCuInSe2 d 1 nCu msolid Cu solid 1 nIn mIn 1 qEV ,

(4)

DHf sa, qd DEsa, qd 1 nCu mCu 1 nIn mIn 1 qeF , (5) and where eF eFa 2 EV , mCu maCu 2 msolid Cu , . Here E is defined as E mIn maIn 2 msolid V V In sNd sN21d sNd 1 eVBM , where E0 ; EsCuInSe2 d is E0 2 E1 the ground state total energy of the N-electron neutral sN21d is the total energy of the CuInSe2 with system and E1 a hole in the VBM and an electron in the reservoir with an energy eVBM equal to the valence-band maximum (VBM) eigenvalue. There are some thermodynamic limits to sm, eF d: eF is bound between the VBM and the conduction-band minimum (CBM), and hmCu , mIn j are bound by (i) the values that will cause precipitation of solid elemental Cu, In, and Se, so mCu # 0,

mIn # 0,

mSe # 0 ,

(6)

(ii) by the values that maintain a stable CuInSe2 compound, so mCu 1 mIn 1 2mSe DHf sCuInSe2 d ,

(7)

where DHf sCuInSe2 d 21.97 eV is the calculated formation energy of solid CuInSe2, and (iii) by the values that will cause formation of binaries, so 2mIn 1 3mSe # DHf sIn2 Se3 d , 2mCu 1 mSe # DHf sCu2 Sed ,

(8)

where our calculated DHf stetragonal In2 Se3 d 22.07 eV [8] and DHf sCu2 Sed 20.31 eV, respectively. Figure 1 gives the calculated “stability triangle” in the twodimensional smCu , mIn d plane as defined by Eqs. (6) and (7). The vertices are A (the Cu-rich and In-rich limit), B (the Cu-poor and In-rich limit), and C (the Cu-rich and In-poor limit). Equation (8) defines the regions where In2Se3 and Cu2Se are stable. We calculated DHf sa, qd for a VCu , VIn , InCu , CuIn , and interstitial Cu sCui d using a 32-atom supercell and a uniform jellium background where q fi 0. The total energies are calculated using the LDA as implemented by the general potential linearized augmented plane wave (LAPW) method [9]. We used Ceperley-Alder exchange correlation potential [10] as parametrized by Perdew and Zunger [11]. The core states are treated relativistically, while the valence states are treated nonrelativistically. The LDA error on the band gap is corrected by adding a constant potential to the conduction states so that the band 4060

FIG. 1. The calculated stability triangle of the Cu-In-Se systems [Eqs. (6) and (7)] in the hmCu , mIn j plane. The vertices correspond to (A) Cu-rich, In-rich; (B) Cu-poor, In-rich; and (C) Cu-rich, In-poor, respectively.

gap of CuInSe2 matches the experimental value of 1.04 eV [7]. The atomic positions were fully relaxed for the q 0 charge state, but no further relaxation was attempted for q fi 0. We estimated that the error in our calculated defect formation energies is 60.2 eV per defect. Figure 2 shows the defect formation energy DHf sa, qd for single defects as a function of the electron Fermi energy eF at the chemical potential values A, B, and C denoted in Fig. 1. The solid dots denote points where the slope of DHf sa, qd vs q changes; the corresponding value of eF is the defect transition energy Ea sqyq0 d. Figure 2 shows the following: (i) The formation energies of single neutral defects 0 d in CuInSe2 are extraordinarily low, e.g., DHf sVCu 0 21.2 eV (at B) and DHf sCuIn d 20.3 eV (at C). In

FIG. 2. Formation energies [Eq. (5)] of VCu , InCu , and CuIn as a function of the electron Fermi energy eF at chemical potentials A, B, and C as shown in Fig. 1. Charge state q determines the slope of each line segment. The shaded area highlights negative formation energies.

VOLUME 78, NUMBER 21

PHYSICAL REVIEW LETTERS

particular, the formation energy of the neutral Cu vacancy is significantly lower than the vacancy formation energies for cations in II-VI’s. There are two reasons (“ionic” and “covalent”) for this. First, Cu is monovalent, while cations in II-VI’s are divalent, so the pointion (Madelung) contribution to the removal energy of the cation is larger in II-VI’s. Second, the covalent Cu-Se bond is easier to break than that of Zn-Se because the Cu 4p energy is higher than the Zn 4p energy (thus the Cu-Se bond is less covalent). Furthermore, the formation of sp 3 hybrids costs more energy in CuInSe2. This is so because the high-lying Cu 3d orbital (relative to the Zn 3d orbital) repels the Se 4p orbital to higher energy [12], thus raising the Se 4s ! 4p promotion energy. (ii) Several low-energy point defects of opposite charges exist at the same eF and m. This allows the formation of charge-compensated defect pairs of low energies, listed in Table I. Notable in Table I is the low formation energy 0 0 1 InCu d of 21.74 eV at point B. neutral pair s2VCu The formation energy of the noninteracting defect pairs can be lowered considerably through interaction and ordering: (a) Interaction: The interaction energy dHint between the component of an isolated pair [Eq. (1)] is calculated as the difference DHf sa 1 bd 2 DHf sad 2 DHf sbd (using the 32-atom supercell [13]). Total energy minimization shows that (Table I) dHint is 24 to 21 eV. We have analyzed the physical origins of dHint by breaking it 2 21 1 InCu d, for example, into recognizable terms. For s2VCu we find dHint 23.45 eV with three contributions: (i) the transfer of two electrons from the high-energy donor level to low-energy acceptor level releases ,21.0 eV (see Fig. 2) and produces charged defect components, (ii) a strong electrostatic attraction between the ensuing charged defects releases ,21.5 eV, and (iii) atomic relaxations upon pairing releases 20.9 eV. The equilibrium geometry of the pair is shown in Fig. 3, where two Cu vacancies are fcc nearest neighbors to the InCu antisite. This arrangement maximizes the point-ion interactions. Furthermore, it lowers the strain: The atomic radius of In is about 23% larger than that of Cu, therefore the pairing of InCu with Cu vacancies reduces the strain energy.

26 MAY 1997

(b) Ordering: Defect pairs whose components are charged may order in the lowest electrostatic Madelung energy configuration. Indeed, we found that the directly calculated LAPW ordering energies scale with the Madelung ordering energies of the same charged defect pair arrays. We thus searched for the lowest-energy array made of 2 21 1 InCu d units by considering a large number of s2VCu ordered configurations, using a simple point-ion model. The lowest energy configuration found forms a tetragonal superstructure with lattice vectors along the f110g, f112g, and f112g directions, respectively, resulting in a Cu 2 VCu 2 InCu 2 VCu f110g superlattice (which can also be viewed as f001g stacking of the vacancy planes). The pair-pair ordering energy dHord sn, m 1d (Table I) for the most stable structure was then calculated by subtracting from the LAPW energy of the defect array the en2 ergy of the isolated s2VCu 1 In21 Cu d pair. dHord sn, m 1d depends on n with an average value of 20.8 eV. We can see from Table I that the sum of interaction and ordering energies dHint 1 dHord of Eq. (1) for the de2 fect pair array s2VCu 1 In21 Cu d is about 24.25 eV, which cancels most of the (positive) formation energy of the iso0 0 d 1 DHf sInCu d 4.26 eV lated, neutral pair: 2DHf sVCu at A. Table II shows the formation energies DHf sn, m 2 21 1d for a few ordered arrays of s2VCu 1 InCu d for the chemical potentials A, B, and C, respectively. We see that a spontaneous formation of stable defect arrays is predicted. The arrows in Fig. 1 point to the chemical potential domains where these ordered defect arrays will be thermodynamically stable. The results of Table II and Fig. 1 can be used to understand the peculiar Cu-In-Se structures known [6] to exist. They can be divided into two classes: those that are on the Cu2Se-In2Se3 tie line [i.e., the compound that can be written as sCu2 Sedx sIn2 Se3 d12x with 0 # x # 1] and those that are not. We predict the stability of all observed tieline compounds as resulting from the repetition of m units

TABLE I. The calculated formation energies DHnon DHf sad 1 DHf sbd (in eV) of noninteracting neutral defects, the intrapair interaction energies dHint , and the pair-pair ordering energies dHord sn, m 1d at chemical potentials A, B, and C as shown in Fig. 1. 0 0 0 0 0 2VCu 1 InCu Cu0In 1 2Cu0i VCu 1 Cu0i InCu 1 CuIn

DHnon dHint dHord

4.26sAd 21.74sBd 6.26sCd 23.45 ,20.8

6.07sAd 12.07sBd 4.07sCd 22.61 ···

2.93sAd 2.93sBd 2.93sCd 21.13 ···

4.47sAd 4.47sBd 4.47sCd 23.67 ···

2 FIG. 3. The calculated structural model for the s2VCu 1 In21 Cu d defect pair.

4061

VOLUME 78, NUMBER 21

PHYSICAL REVIEW LETTERS

TABLE II. Calculated formation energies DHf sn, m 1d DHnon smd 1 dHint 1 dHord sn, m 1d [Eq. (2)] (in eV) of the 2 21 ordered arrays of n units of s2VCu 1 InCu d for every m unit of CuInSe2. dHord sn, m 1d are 20.76, 20.78, and 20.79 eV for n 4, 5, and 6, respectively, while dHint and DHnon smd are taken from the first column of Table I. CuIn5Se8 CuIn3Se5 Cu3In7Se12

n

mA

mB

mC

4 5 6

0.05 0.03 0.02

25.95 25.97 25.98

2.05 2.03 2.02

2 of s2VCu 1 In21 Cu d for every n unit of CuInSe2. These are CuIn5Se8 (n 4, m 1), CuIn3Se5 (n 5, m 1), Cu2In4Se7 (n 7, m 1), Cu3In5Se9 (n 9, m 1), and Cu7In19Se32 (n 16, m 3). Electron diffraction data on CuIn3Se5 [14] suggest f001g stacking of the vacancies, in agreement with our calculations. There are three off-the-tie-line compounds that are observed [6] but not accounted for by the above argument: CuIn7Se12, Cu4In9Se16, and Cu3In6Se11. In light of the low formation energy of neutral Cu vacancy (Fig. 2), we can rationalize the stabilities of these three compounds as emerging from the creation of 2, 1, and 1 Cu vacancies per molecule in the (tie-line) compounds Cu3In7Se12 (n 6, m 1), Cu5In9Se16 (n 8, m 1), and Cu4In6Se11 (n 11, m 1), respectively. To understand why CuInSe2 exhibits a surprising electric tolerance to its .1% structural point defects, we calculated the electronic structure of an isolated, interacting 2 1 In21 s2VCu Cu d pair. All the deep defect levels of VCu and InCu (which act as the recombination centers) are removed from the band gap due to pairing. We also find that, when the defect array orders, the (LDA-corrected) band gaps of the “ordered defect compounds” CuIn5Se8, CuIn3Se5, and Cu3In7Se12 are 1.38, 1.29, and 1.23 eV, respectively, all larger than the 1.04 eV band gap of CuInSe2. This explains the surprising electrical tolerance of nonstoichiometric CuInSe2 to its structural defects [7]. In summary, the key factors that stabilize spontaneous defect-pair formation and ordering in CuInSe2 are (i) the ability to form charge-compensating defects solely on the cation sublattices (thus, the need for two heterovalent cations), (ii) the low metal vacancy formation energy

4062

26 MAY 1997

(thus, the need for low-valent cations with possibly active d orbitals), and (iii) the large interdefect electrostatic interactions (thus, the need for partially ionic systems). This work was supported by the U.S. Department of Energy, DOE-EERE under Contract No. DE-AC3683CH10093.

[1] S. B. Zhang and J. E. Northrup, Phys. Rev. Lett. 67, 2339 (1991). [2] G. A. Baraff and M. Schluter, Phys. Rev. B 33, 7346 (1986). [3] D. B. Laks et al., Phys. Rev. B 45, 10 965 (1992); C. Van De Walle (private communication). [4] J. L. Shay and J. H. Wernick, Ternary Chalcopyrite Semiconductors (Pergamon, Oxford, 1975). [5] Composition-preserving antisite pairs are trivial cases, where the formation of an array does not cost any energy, e.g., zinc-blende GaAs can be viewed as a 50%-50% solid made of antisite pairs GaAs 1 AsGa . Here, we will discuss cases other than the antisite pair arrays. [6] P. Villars and L. D. Calvert, Pearson’s Handbook of Crystallographic Data for Intermetallic Phases (ASM International, Materials Park, Ohio, 1991), p. 2884. [7] Copper Indium Diselenide for Photovoltaic Applications, edited by T. J. Coutts, L. L. Kazmerski, and S. Wagner (Elsevier, Amsterdam, 1986). [8] Here, we will not consider hexagonal In2Se3, despite the fact that its calculated energy is about 1.1 eV lower. We expect that decomposition of (tetragonal) CuInSe2 produces initially tetragonal In2Se3 which is inhibited by an activation barrier from transforming into the hexagonal phase. [9] S.-H. Wei and H. Krakauer, Phys. Rev. Lett. 55, 1200 (1985). [10] D. M. Ceperly and B. J. Alder, Phys. Rev. Lett. 45, 566 (1980). [11] J. P. Perdew and A. Zunger, Phys. Rev. B 23, 5048 (1981). [12] S.-H. Wei and A. Zunger, Phys. Rev. B 37, 8958 (1988). [13] We assume that the long-range Coulomb interactions 2 and In21 among charged VCu Cu dominate the cell-cell interaction. Using a dielectric constant of e 16 [7], 2 1 In21 the cell-cell interaction of s2VCu Cu d in the 32-atom supercell is estimated to be less than 60.1 eV. [14] H. Z. Xiao, L.-Chung Yang, and A. Rockett, J. Appl. Phys. 76, 1503 (1994).